Lead-free high-temperature dielectrics with wide operational range
Robert Dittmer, Wook Jo, Dragan Damjanovic, and Jürgen Rödel
Citation: Journal of Applied Physics 109, 034107 (2011); doi: 10.1063/1.3544481 View online: http://dx.doi.org/10.1063/1.3544481
View Table of Contents: http://scitation.aip.org/content/aip/journal/jap/109/3?ver=pdfcov Published by the AIP Publishing
Articles you may be interested in
Effect of composition on electrical properties of lead-free Bi0.5(Na0.80K0.20)0.5TiO3-(Ba0.98Nd0.02)TiO3 piezoelectric ceramics
J. Appl. Phys. 114, 027005 (2013); 10.1063/1.4811813
High T c lead-free Ba Ti O 3 – ( Bi 1 ∕ 2 Na 1 ∕ 2 ) Ti O 3 positive temperature coefficient of resistivity ceramics with electrically heterogeneous structure
Appl. Phys. Lett. 91, 162904 (2007); 10.1063/1.2799878
Phase structure, microstructure, and electrical properties of bismuth modified potassium-sodium niobium lead-free ceramics
J. Appl. Phys. 102, 054102 (2007); 10.1063/1.2775997
Dielectric behavior and microstructure of ( Bi 1 ∕ 2 Na 1 ∕ 2 ) TiO 3 – ( Bi 1 ∕ 2 K 1 ∕ 2 ) TiO 3 – BaTiO 3 lead-free piezoelectric ceramics
J. Appl. Phys. 97, 104101 (2005); 10.1063/1.1890453
Electromechanical and ferroelectric properties of ( Bi 1 ∕ 2 Na 1 ∕ 2 ) TiO 3 – ( Bi 1 ∕ 2 K 1 ∕ 2 ) TiO 3 – BaTiO 3 lead-free piezoelectric ceramics
Appl. Phys. Lett. 85, 91 (2004); 10.1063/1.1767592
Lead-free high-temperature dielectrics with wide operational rangeRobert Dittmer,1Wook Jo,1,a兲Dragan Damjanovic,2and Jürgen Rödel1
Institute of Materials Science, Technische Universität Darmstadt, Petersenstr. 23, 64287 Darmstadt, Germany
Ceramics Laboratory, Swiss Federal Institute of Technology, EPFL, 1015 Lausanne, Switzerland
共Received 25 October 2010; accepted 10 December 2010; published online 9 February 2011兲 The dielectric, electrical and structural properties of 共1 –x兲共0.94Bi1/2Na1/2TiO3– 0.06BaTiO3兲–
xK0.5Na0.5NbO3 共BNT– BT–xKNN兲 with x= 0.09, 0.12, 0.15, and 0.18 were investigated as potential candidates for high-temperature capacitors with a working temperature far beyond 200 ° C. Temperature dependent dielectric permittivity 共兲 showed two local broad maxima that at the optimal composition of KNN共x= 0.18兲are combined to form a plateau. This then results in a highly temperature-insensitive permittivity up to⬃300 ° C at the expense of a small reduction in absolute permittivity values. High-temperaturein situx-ray diffraction study showed pseudocubic symmetry without obvious structural changes, which implies that the dielectric anomalies observed could only be a consequence of a slight change in space group. BNT–BT–0.18KNN showed a permittivity of ⬃2150 at the frequency of 1 kHz at 150 ° C with a normalized permittivity /150 °C varying no more than⫾10% from 43 to 319 ° C. With very good electrical properties persisting up to 300 ° C, i.e., a resistivity on the order of magnitude of 108 ⍀m and the RC constant of about 1 s, the
examined BNT– BT–xKNN compositions present a good starting point for the development of high-temperature capacitor materials. ©2011 American Institute of Physics.
关doi:10.1063/1.3544481兴 I. INTRODUCTION
Capacitors are indispensable components for passive parts in contemporary electronic devices. They fulfill a vari-ety of important functions including voltage smoothing, pulse discharge, filtering, dc blocking, coupling, decoupling, snubbing, and power conditioning.1,2However, with increas-ing demands on the performance and efficiency of electronic systems, the requirements on capacitor materials imposed by the industries are increasing as well. The high-temperature electronics are of particular interest as control units are in-tended to be placed close to hot components, such as engines or transmissions.3,4 This allows a higher degree of integra-tion, and thereby simplifies the assembly of the overall prod-uct 共e.g., the vehicle兲 and saves cost and mass of thermal insulation and wiring. For their contribution to miniaturiza-tion, cost-effectiveness and lightweight design, high-temperature electronics are highly desired in automotive, aerospace, and defense technologies.5,6In automotive indus-try the trend toward hybrid or electrically powered cars is pushing the temperature envelope even higher due to the increased integration of power electronics and the heat dis-sipation thereof. Other applications where electronics are re-quired to operate at elevated temperatures include instrumen-tation for geothermal wells, oil well logging, and nuclear reactors.4,5
In all these applications, the electric components have to operate under harsh conditions while maintaining good elec-trical properties and providing high reliability at tempera-tures beyond 200 ° C. Among the required passive devices, the capacitor is probably one of the most challenging
com-ponents. Materials are chosen for high permittivity at their phase transition with the attendant disadvantage that tem-perature dependence is high at these temtem-peratures.7 How-ever, a capacitor must operate with a relatively constant ca-pacitance over the whole operational range. Moreover, a high permittivity is needed in order to make a large value capaci-tor, which is required for power conditioning circuits.5If the volumetric efficiency of the dielectrics is too low, the capaci-tor becomes too large, and hence ill-suited for system min-iaturization, or may even fail due to thermal stresses induced during thermal cycling. The development of a high-temperature capacitor is further impeded by resistivity and loss factor that also exhibit a strong dependence on tempera-ture. A capacitor suited for high-temperature applications is required to exhibit high resistivity and low losses. Another constraint is the demand for low frequency dispersion of the capacitance and the loss factor. In addition to these technical requirements, the production of a mass market product like a capacitor has to be cost-effective. Therefore, the use of rare raw materials or unconventional production methods is not suitable for fabrication on a large scale.
Dielectrics that show good electrical properties at room temperature usually exhibit strongly reduced properties at elevated temperatures and thus are often limited to tempera-tures below 125 ° C.8,9 Other dielectrics feature very high operational temperatures but either lack high permittivity or suffer from strong temperature dependence.10–12 Bridger et al.13 showed that 0.9共Bi1/2Na1/2兲TiO3– 0.1KTaO3 exhibits a
relatively flat permittivity from 80 to 260 ° C though permit-tivity outside this range rapidly decreases. Limet al.14have shown that the BiScO3– BaTiO3–共K1/2Bi1/2兲TiO3 共BSBT–
KBT兲pseudoternary system exhibits good electrical proper-ties over a wide temperature range. However, the large
fre-a兲Electronic mail: firstname.lastname@example.org.
0021-8979/2011/109共3兲/034107/5/$30.00 109, 034107-1 © 2011 American Institute of Physics
quency dispersion at low temperatures presents a serious drawback. Moreover, BSBT–KBT incorporates the element scandium which is also found in other materials that had been suggested for high-temperature dielectrics.15,16The ex-traordinarily high price of scandium, however, limits the use of such materials to academic research. With regard to a potential application, it is vital to incorporate only those raw materials that are widely available with a reasonable price.
Zhang et al.17 investigated 共Bi1/2Na1/2兲TiO3– BaTiO3–
共K0.5Na0.5兲NbO3 共BNT–BT–KNN兲 pseudoternary systems
mainly with respect to high electric field properties. Thereby, it was discovered that electric field induced phase changes cause large strain behavior in compositions with low KNN-content rendering them suitable for actuators. Materials with higher amounts of KNN were found to exhibit high electros-trictive constants and temperature-insensitive field-induced strain which are attractive for high-precision positioning de-vices and other actuators.18
In this study, we report the electric and dielectric prop-erties of 共1 –x兲关0.94BNT– 0.06BT兴–xKNN with x= 0.09, 0.12, 0.15, and 0.18. The influence of the KNN-content on permittivity, loss factor, resistivity and structure was investi-gated for temperatures from 30 up to 400 ° C. We demon-strate that this material is promising as a dielectric for high-temperature applications owing to its very good dielectric and electric characteristics that can be achieved over a very broad operational temperature range.
Ceramics were produced via a mixed oxide route using reagent grade oxides and carbonates 共Alfa Aesar GmbH & Co. KG, Karlsruhe, Germany兲. First, Bi2O3 共99.975%兲,
Na2CO3 共99.5%兲, TiO2 共99.9%兲, BaCO3 共99.8%兲, K2CO3
共99.0%兲, and Nb2O5 共99.9%兲 were mixed according to the
stoichiometric formula and milled in a planetary ball-mill共Fritsch Pulverisette 5, Idar-Oberstein, Germany兲for 24 h at 250 rpm with zirconia balls in ethanol. After drying at 100 ° C, the mixed powder was calcined at 900 ° C for 3 h, and subsequently ball-milled again for 24 h. Pestled and sieved powders were compacted into pellets of 10 mm in diameter. To facilitate the densification, powder compacts were hydrostatically pressed under 300 MPa. Sintering was performed at 1100 ° C for 3 h in a covered alumina crucible with atmospheric powder of the same composition to mini-mize the loss of volatile elements. Finally the sintered pellets were ground, and polished. Samples were electroded with a silver paint on both sides and fired at 400 ° C for 30 min.
Dielectric measurements were carried out with a HP4192A impedance analyzer 共Hewlett-Packard Co., Pala Alto, CA, USA兲 using a Nabertherm LE4/11/R6 furnace 共Nabertherm GmbH, Lilienthal, Germany兲 with a home-made sample holder at a heating rate of 2 K min−1. The
leakage current was measured by means of a Keithley 6517B high resistance meter and a home-made furnace at a ramping rate of 4 K min−1 up to 400 ° C under a dc voltage of 60 V.
The RC constant was calculated from the capacitance at 1 kHz and the dc resistance.
Density was determined via the Archimedes method. For
the microstructural analysis, samples were polished with dia-mond paste down to 0.25 m and coated with a thin layer of carbon for subsequent observation in the scanning electron microscope L30 FEG/ESEM 共Philips/FEI, Hillsboro, OR, USA兲. The average grain size was determined from the mean intercept length multiplied by 1.56. Room temperature struc-ture was characterized by a powder x-ray diffraction共XRD, STADI P STOE, Darmstadt, Germany兲 with a transmission geometry using CuK␣1 radiation. To release stress induced
during the sample preparation stage, the crushed powders were thermally annealed at 400 ° C for 1 h. For the tempera-ture dependent structural analysis, a reflective XRD appara-tus 共Bruker AXS D8, Karlsruhe, Germany兲equipped with a furnace was employed using CuK␣radiation.
III. RESULTS AND DISCUSSION
Figure 1 illustrates a segment of the pseudo-ternary phase diagram of the BNT-BT-KNN system showing the lo-cation of the four compositions examined. These are 共1 –x兲 ⫻关0.94BNT– 0.06BT兴–xKNN with x= 0.09, 0.12, 0.15, and 0.18, which will be termed 9KNN, 12KNN, 15KNN, and 18KNN in the following. Note that all four compositions are a derivative of the base composition 0.94BNT–0.06BT, which lies at the morphotropic phase boundary between rhombohedral BNT and tetragonal BT.19 Using room-temperature XRD, it was confirmed that all four composi-tions were successfully synthesized as single phase materials that show pseudocubic structure.
The average grain size G and the relative densityof the materials studied are summarized in TableI. The KNN con-tent has little influence both on the density and on the aver-age grain size. All four specimens showed a very homoge-neous microstructure with practically the same average grain
FIG. 1. 共Color online兲Illustration of the compositions studied.
TABLE I. Average grain size, G, and relative density,. G 共m兲 共%兲 9KNN 0.5⫾0.1 98⫾0.5 12KNN 0.5⫾0.1 98⫾0.3 15KNN 0.6⫾0.1 98⫾0.7 18KNN 0.5⫾0.1 96⫾0.3
034107-2 Dittmeret al. J. Appl. Phys.109, 034107共2011兲
size of ⬇0.5 m, and the relative density of ⬎96%. The fact that fairly dense specimens with submicron-sized grains are available by a conventional sintering technique in the current system is highly promising from the industrial point of view, since it is an essential prerequisite for mass produc-tion and miniaturizaproduc-tion of multilayer ceramic capacitors.
Figure 2 provides the temperature dependent dielectric permittivity and loss factor from room temperature up to 400 ° C for all the compositions studied. Two distinctive di-electric anomalies are discerned common to BNT-based materials.20 The first dielectric anomaly at ⬇100 ° C in-volves a frequency dependent dielectric permittivity, which is known as one of the distinctive features characterizing relaxor ferroelectrics.21–23In fact, the changes in loss tangent also support the assumption that the material has relaxor characteristic.24 The other dielectric anomaly appears at ⬇250 ° C showing neither frequency dispersion nor abrupt changes in loss factor. Comparison of the plots for all the compositions investigated clearly rationalizes the effect of KNN which is to render the permittivity values insensitive to temperature. Here, the temperatures that designate the first and the second dielectric anomaly are referred to as Tm1and
Tm2, respectively, and are summarized in Fig. 3. It is
dem-onstrates that Tm1 decreases while Tm2 increases with
in-creasing KNN content. At the same time, the permittivity values at both temperatures are reduced. The increase in
⌬T共=Tm2− Tm1兲and the reduction in the permittivity values are responsible for the expansion of the range of working temperature and for the temperature insensitivity, respec-tively. Feasibility of the studied materials as high tempera-ture dielectrics is further quantified in Fig.4
The permittivity normalized to the permittivity at 150 ° C /150 °C is plotted at 1 kHz. The dotted and the
dashed frames indicate the operational ranges with⫾5% and
⫾10% tolerance, respectively. For⫾5% tolerance the opera-tional range increases from 109– 292 ° C to 53– 294 ° C. This is a remarkably flat progression of the permittivity con-sidering that there is less than 5% variation in a range that spans over 240 K, reaching almost 300 ° C in 18KNN. For a
⫾10% tolerance the working temperature spans from 96– 313 ° C in 9KNN to 43– 319 ° C in 18KNN. This small deviation in permittivity is a notable feature since the Elec-tronic Industries Alliance 共EIA兲 permits ⫾15% deviations for commercially available X7R capacitors that are currently designated for operation at elevated temperatures.
Albeit limited to 125 ° C, those X7R materials exhibit advantages at low temperatures down to −55 ° C. In contrast, the permittivity of the materials presented here decreases gradually when the temperature drops below Tm1. Therefore,
it would be beneficial to shift Tm1below room temperature, e.g., by means of additional chemical substitutions. This
FIG. 2. 共Color online兲Permittivity and loss factor for共a兲9KNN,共b兲12KNN,共c兲15KNN, and共d兲18KNN at different frequencies.
FIG. 3. 共Color online兲Evolution of characteristic temperatures and permit-tivity values with KNN content共data at 1 kHz, Tm1and Tm2derived from
first derivative of permittivity兲.
FIG. 4. 共Color online兲Change in permittivity at 1 kHz共at 150 ° C兲and illustration of operational range for deviation of⫾5%共dotted frame兲and
⫾10% 共dashed frame兲 for 共a兲 9KNN, 共b兲 12KNN,共c兲 15KNN, and 共d兲 18KNN.
could not only expand the operational temperature range but potentially also may eliminate the frequency dispersion at room temperature.
High permittivity, temperature stability, and low loss are not the only key figures; for the application as a capacitor, the dielectric material is required to have both high resistiv-ity and RC constant even at elevated temperatures. Although an ideal capacitor would have an infinite resistivity, all real capacitors have a finite value for its resistivity. Hence, a charged capacitor will have a leakage current and will dis-charge through its own resistance. Because of this, a capaci-tive device of higher performance is obtained by higher resistivity.25Figure5illustrates that resistivity is very similar among the four BNT–BT–KNN materials from 100 to 400 ° C.
Compared with soft PZT, which has a resistivity in the order of magnitude of 1012 ⍀m at room temperature, the resistivity obtained for the BNT–BT–KNN materials at 100 ° C is comparably high as it lies in the range of 1011– 1012 ⍀m.7
For all compositions, the resistivity drops exponentially showing Arrhenius behavior with predomi-nantly linear curves in the logarithmic plot against inverse absolute temperature. The activation energyEafor the
elec-trical conductivity is 0.82 eV 共9KNN兲, 0.74 eV 共12KNN兲, 1.04 eV共15KNN兲, and 0.77 eV共18KNN兲in the range from 100 to 300 ° C. At 300 ° C the resistivity is in the order of magnitude of 108 ⍀m, outperforming PZT5A with 1.9
⫻107 ⍀m, 0.36BiScO
3– 0.64PbTiO3 共BSPT64兲 with 2.4
⫻106 ⍀m or 共Pb, Ba兲Nb
2O6 with 105 ⍀m.7,16
The time dependence of a discharging process of a ca-pacitor is determined by the time constantaccording to Eq.
HereQ共t兲is the charge at timetandQ0is the initial charge. The time constantis defined as
with the resistance Rand the capacitance C. Att=the ca-pacitance drops to e−1共⬇37%兲of the initial value, and hence
RC is a measure for the quality of a material to maintain its
charge. Therefore, a highRC value is synonymous for high capacitance and high resistance at the same time. Figure 6
provides a comparison of the RC value at 300 ° C for four BNT–BT–KNN compositions with reference to other poten-tial candidates for high temperature dielectrics.
The addition of KNN reduces theRCconstant at 300 ° C from 2.64 s for 9KNN to 1.13 s for 18KNN. These values are comparably high surpassing those of other materials such as 0.8共0.4BiScO3– 0.6BaTiO3兲– 0.2共Bi1/2K1/2兲TiO3 共BSBT–
20BKT兲, PZT5A or BSPT64. The highRC values of BNT– BT–KNN outperform materials with toxic elements such as lead or expensive elements such as scandium and beyond that BNT–BT–KNN features the aforementioned high per-mittivity over a broad temperature range. Tailoring both re-sistivity andRCconstant further by dopants as already dem-onstrated for other material systems is encouraged for the future.16,26,27
As already discussed, the reason behind the broad pla-teau in temperature dependent permittivity appears to be due to two distinct dielectric anomalies that are gradually smeared into each other as KNN content increases. Of course, the physical origin behind these two anomalies has to be clarified in order to fully understand and further optimize these materials. A similar characteristic of 共T兲 is already known from the parent pseudobinary BNT–BT system, which also shows two nearby local maxima though very dif-ferent in magnitude.19,28
High-temperature in situXRD measurements were per-formed from room temperature up to 300 ° C for 18KNN. No obvious noncubic distortion was detected within the ana-lyzed temperature range. However, the changes in intensity indicate that there are at least two successive structural changes taking place. Note that a discontinuous change in the intensity of共110兲pcpeak共the subscript “pc” here refers to
pseudocubic兲 is clearly seen in the temperature range of about 150– 240 ° C in Fig.7.
Hintersteinet al.29 demonstrated by combining neutron with XRD techniques that the introduction of KNN to BNT– 6BT stabilizes the high temperature P4bm phase at room temperature, the lattice distortion of which is so small关c/a FIG. 5. 共Color online兲Resistivity as function of inverse absolute
tempera-ture measured at 60 Vdc. FIG. 6.共Color online兲Comparison of time constants at 300 ° C with BSBT–
20BKT共Ref.14兲, PZT5A共Ref.16兲, BiSrTiO4共Ref.14兲, BiTiO3共Ref.14兲, BSPT64共Ref.16兲, and commercial X7R共Ref.14兲.
034107-4 Dittmeret al. J. Appl. Phys.109, 034107共2011兲
⬇1.000共3兲兴that the phase can only be assigned to be tetrag-onal from the presence of superlattice reflection, which is properly detectable only by neutron diffraction. In addition, Webber et al.30 showed that there is an additional phase
P4/mbm共or P4/mmm兲, which is paraelectric but ferroelas-tic, between the tetragonalP4bmand the cubicPm¯m3 in the BNT–6BT system. It is thus suggested that the structural evolution in 18KNN is given in terms of the XRD length scale as P4bm共FE/FEla兲 → ⬃160 °C P4/mbm共PE/FEla兲 → ⬃250 °C Pm¯m3 共PE/PEla兲,
where FE, PE, FEla, and PEla denote ferroelectric, paraelectric, ferroelastic, and paraelastic, phases, respec-tively. It is interesting to note that though the first dielectric anomaly of 18KNN共see Fig.2兲is observed below 100 ° C, the fact that no obvious structural change is observed from thein situXRD study strongly supports the assumption that BNT–BT–KNN is a relaxor.22It is interesting to note that the actual structure change implied by the XRD study at about 160 ° C is closely correlated with the temperature regime where dielectric dispersion disappears with an inflection point in the temperature-dependent dielectric permittivity data. However, any physical reasoning for the correlation warrants further systematic investigations.
Potential compositions for high temperature dielectric applications were developed in a pseudoternary lead-free BNT–BT–KNN system. These commercially viable cost-effective materials provide not only temperature insensitivity but also a wide operational temperature range. Among the studied compositions, 18KNN was shown to offer⬎270 ° C 共from 43 to 319 ° C兲 of reliable operation temperature win-dow and⌬/150 °C⬍10% with concurrent permittivity
val-ues exceeding 2000. Furthermore, its resistivity is compara-tively high throughout the measured temperature range with anRC constant of about 1 s at 300 ° C. We suggest that the materials presented render a good starting point for the de-velopment of high-capacitance, cost-effective capacitors for high-temperature application beyond 200 ° C.
This work was financially supported by the Deutsche Forschungsgemeinschaft共DFG兲under SFB 595/A1.
1C. A. Randall, H. Ogihara, J.-R. Kim, G.-Y. Yang, C. S. Stringer, S.
Trolier-McKinstry, and M. Lanagan, Proceedings of the IEEE Pulsed Power Conference 2009, Washington, DC, 28 June–2 July 2009, p. 346.
2A. Nishino,J. Power Sources60, 137共1996兲.
3A. N. Hammoud and I. T. Myers, Proceedings of the Annual Report
Con-ference on Electrical Insulation and Dielectric Phenomena, Leesburg, VA, 29 October–2 November 1989, p. 459.
4R. S. Demcko, Proceedings of the IEEE Electronics Components
Confer-ence, Los Angeles, CA, 9–11 May 1988, p. 390.
5R. R. Grzybowski and B. Gingrich,ASME J. Eng. Gas Turbines Power 121, 622共1999兲.
6R. W. Johnson, J. L. Evans, P. Jacobsen, J. R. Thompson, and M.
Chris-topher,IEEE Trans. Electron. Packag. Manuf.27, 164共2004兲.
7T. R. Shrout, R. Eitel, and C. A. Randall, inPiezoelectric Materials in
Devices, edited by N. Setter共EPFL, Swiss Federal Institute of Technology,
Lausanne, 2002兲, p. 413.
8Y. Yuan, S. R. Zhang, X. H. Zhou, B. Tang, and B. Li,J. Electron. Mater. 38, 706共2009兲.
9T. Li, L. T. Li, Y. Kou, and Z. L. Gui,J. Mater. Sci. Lett.19, 995共2000兲. 10H. Beltrán, N. Maso, E. Cordoncillo, and A. R. West,J. Electroceram.18,
11A. Yializis, G. L. Powers, and D. G. Shaw,IEEE Trans. Compon.,
Hy-brids, Manuf. Technol.13, 611共1990兲.
12C. J. Stringer, T. R. Shrout, and C. A. Randall,J. Appl. Phys.101, 054107
13K. Bridger, A. V. Cooke, and W. A. Schulze, U.S. Patent No. US7,697,263
B2共13 April 2010兲.
14J. B. Lim, S. J. Zhang, N. Kim, and T. R. Shrout,J. Am. Ceram. Soc.92,
15H. L. Du, W. C. Zhou, F. Luo, D. M. Zhu, S. B. Qu, Y. Li, and Z. B. Pei,
J. Appl. Phys.104, 044104共2008兲.
16S. Zhang, E. F. Alberta, R. E. Eitel, C. A. Randall, and T. R. Shrout,IEEE
Trans. Ultrason. Ferroelectr. Freq. Control52, 2131共2005兲.
17S. T. Zhang, A. B. Kounga, E. Aulbach, H. Ehrenberg, and J. Rödel,Appl.
Phys. Lett.91, 112906共2007兲.
18S. T. Zhang, A. B. Kounga, W. Jo, C. Jamin, K. Seifert, T. Granzow, J.
Rödel, and D. Damjanovic, Adv. Mater.21, 4716共2009兲.
19T. Takenaka, K. Maruyama, and K. Sakata,Jpn. J. Appl. Phys., Part 130,
20F. Cordero, F. Craciun, F. Trequattrini, E. Mercadelli, and C. Galassi,
Phys. Rev. B81, 144124共2010兲.
21L. E. Cross, Ferroelectrics76, 241共1987兲.
22G. A. Samara,J. Phys.: Condens. Matter15, R367共2003兲. 23A. A. Bokov and Z. G. Ye,J. Mater. Sci.41, 31共2006兲. 24H. Qian and L. A. Bursill,Int. J. Mod. Phys. B10, 2007共1996兲. 25G. Y. Yang, E. C. Dickey, C. A. Randall, D. E. Barber, P. Pinceloup, M. A.
Henderson, R. A. Hill, J. J. Beeson, and D. J. Skamser,J. Appl. Phys.96, 7492共2004兲.
26W. Hofman, S. Hoffmann, and R. Waser,Thin Solid Films305, 66共1997兲. 27D. Dimos, R. W. Schwartz, and S. J. Lockwood,J. Am. Ceram. Soc.77,
28T. Oh and M. H. Kim,Mater. Sci. Eng., B132, 239共2006兲.
29M. Hinterstein, M. Knapp, M. Hölzel, W. Jo, A. Cervellino, and H.
Ehren-berg,J. Appl. Crystallogr.43, 1314共2010兲.
30K. G. Webber, Y. Zhang, W. Jo, J. E. Daniels, and J. Rödel,J. Appl. Phys. 108, 014101共2010兲.
FIG. 7. 共Color online兲The共110兲 reflection for 18KNN remains virtually unchanged from 30 to 300 ° C besides minor fluctuations in intensity and a shift in the reflex due to thermal expansion 共note: diffraction pattern is collected from CuK␣1 and CuK␣2 wavelength兲.